-150-140-130 0

0.01 0.02 0.03 0.04 0.05

Im χ in arb. units

phonons Coulomb total

-90 -80 -70
energy E - E_{G} in meV

0 0.1 0.2 0.3

-30 -20 -10 0 0

1 2 3

s-shell p-shell WL

(a)5×10^{10}cm^{−2}

-160 -150 -140 -0.02

-0.01 0 0.01

Im χ in arb. units

phonons Coulomb total

-100 -90 -80
energy E - E_{G} in meV

0 0.02 0.04 0.06 0.08 0.1 0.12

-30 -20 -10 0 0

0.2 0.4 0.6 0.8

s-shell p-shell WL

(b)2×10^{11}cm^{−2}

**Fig. 6.3: Comparison of carrier-carrier and carrier-phonon contributions to the dephasing**
in room-temperature absorption spectra for QD systems.

the Coulomb interaction is the dominant dephasing mechanism for the QD resonances. For the excitonic resonance of the WL, the two mechanisms are equally important at this rather high carrier density, where the s-shell transition is already in the gain regime.

These results indicate the importance of including both, carrier-carrier and carrier-phonon interaction, on a self-consistent footing in the calculation of optical absorption spectra.

Artifacts that arise from using non-self-consistently calculated single-particle energies as well as a detailed analysis on the relative importance of diagonal and off-diagonal contribu-tions to the dephasing and various scattering channels is presented by Lorke [167], Lorke et al. [168]. Furthermore, this model for the optical absorption of QD systems predicts new physical effects like a reduction of the optical gain with increasing carrier density [169], which can not be observed in QWs and is unique to QD systems. Another application of this model is the calculation of technologically relevant quantities like the line-width-enhancement factor that is important for laser application [170].

In TRPL experiments a pump pulse is used to optically excite carriers into the energetically higher WL or bulk states. Scattering processes due to carrier-carrier and carrier-phonon interaction lead to a relaxation towards the energetically lowest states, resulting in a quasi-equilibrium carrier distribution. From the optically active states carrier recombination processes takes place. For the theoretical description of the corresponding TRPL signal we treat the light-matter interaction quantum-mechanically. The Hamiltonian we consider in the following is given by (3.2), where the dipole interaction with a classical light ﬁeld is replaced by the quantized light-matter interaction

Hˆ_{LM} =−i

ξ,12

g^{ξ}_{12}ˆa^{†}_{1}aˆ_{2}ˆb_{ξ}−h.c.

1= 2 (6.19)

with1 ∈ {α_{1}, λ_{1}}containing state index α and band indexλ. Carrier creation and
anni-hilation operators are denoted by ˆa^{(†)}_{i} and photon operators byˆb^{(†)}_{ξ} . The coupling matrix
element

g_{12}^{ξ} =E^{ξ} 1|e**r**·**U**^{ξ}(r)|2 ≈E_{ξ} **d**λ1λ2 **U**xi δ_{α}_{1}_{α}_{2} =g^{ξ}δ_{α}_{1}_{α}_{2} . (6.20)
contains the overlap of the local dipolese**r**with the optical mode**U**^{ξ}(r)which is classiﬁed
by the indexξ ∈ {q,**e}**denoting the mode**q**and the polarization**e**. This can be simpliﬁed
when considering equal envelope wavefunctions and the dipole approximation (second
term). A detailed discussion of the light-matter interaction Hamiltonian is presented for
example in Refs. [67, 68, 140, 149]. The interaction vertices of the light-matter interaction
are similar to those of the carrier-phonon interaction. A carrier scatters from state |1to
state |2 by emission or absorption of a photon in mode ξ. The main difference is that
the light-matter interaction describes inter-band processes, whereas in the carrier-phonon
interaction only intra-band processes are involved. In this notation the Hamiltonian (6.19)
contains resonant cˆ^{†}vˆˆb as well as non-resonant ˆv^{†}cˆˆb terms. A common approximation
at this point is the so-called rotating-wave approximation (RWA) where one restricts to
resonant terms only, as the non-resonant terms describe elementary processes that are not
energy-conserving.

The quantities of interest for the calculation of the PL are the carrier-populationsf_{α} and
the photon numberN_{ξ} =ˆb^{†}_{ξ}ˆb_{ξ}. The PL spectrum itself is obtained from the total number
of emitted photons,

I(ω) =

ξ

d
dtN_{ξ}

ω=c|q|. (6.21)

To derive the corresponding equations of motion we use the cluster expansion method of Fricke [65, 66], which is introduced brieﬂy in Chap. 3.1. In principle, here one could also introduce a photon Green’s function and solve the corresponding Dyson equation. From the cluster expansion, the resulting equations of motion for the carrier populations and the

photon number are the semiconductor-luminescence equations (SLE) d

dtN_{ξ} =|g_{ξ}|^{2}Re

α

ˆb^{†}_{ξ} ˆv_{α}^{†} cˆ_{α} (6.22)
d

dtf_{α}

LM=−Re

ξ

|g_{ξ}|^{2}ˆb^{†}_{ξ}vˆ_{α}^{†} ˆc_{α}+ d
dtf_{α}

coll

. (6.23)

The number of photons emitted into the modeξis determined by the photon-assisted inter-band transition amplitude, i.e. the recombination of carriers. Correspondingly, the popula-tion of the involved states is reduced by the emission into all modesξ. The photon assisted polarization obeys its own equation of motion

id

dt −(^{c}−^{v}−ω_{ξ}−iΓ)

ˆb^{†}_{ξ} ˆv_{α}^{†} ˆc_{α}=ig_{ξ}f_{α}^{c} (1−f_{α}^{v}) +N_{ξ}(f_{α}^{c} −f_{α}^{v})
+ (f_{α}^{c} −f_{α}^{v})

β

V_{αβαβ} ˆb^{†}_{ξ} ˆv_{β}^{†} ˆc_{β}
+ig_{ξ}

β

C_{βααβ}^{x} (6.24)

containing spontaneous emission (ﬁrst term RHS), stimulated emission which is impor-tant in cavities (second term RHS), and correlation terms. Similar to the SBE, the single-particle energiesare renormalized due to Hartree and Fock contributions of the Coulomb interaction and excitonic resonances in the photoluminescence are found (third term RHS).

The fourth term contains electron-hole correlations.

The electron-hole correlationsC^{x} are two-particle contributions (doublet level) due to the
Coulomb interaction. In contrast, the stimulated emission and the excitonic
renormaliza-tion arise from a factorizarenormaliza-tion of higher order correlarenormaliza-tions likeˆb^{†}ˆb ˆc^{†}ˆc. Note, that the
creation or emission of a photon corresponds to a inter-band carrier-transition and
corre-spondingly expectation values likeˆb^{†}ˆv^{†}cˆ represent two-particle processes. The analysis
of correlations due to light-matter and Coulomb interaction as well as photon-photon
cor-relations is not subject of this thesis. For details we refer the reader to Refs. [67, 68, 140].

Considering additionally the carrier-phonon interaction, the corresponding correlations give rise to a dephasing of the photon-assisted polarization and other correlations. For the calculations presented below we consider at this point a phenomenological dephasing Γ. A more sophisticated approach to include dephasing processes due to carrier-phonon interaction within a microscopic approach is presented in Refs. [171, 172] for QW systems.

Within this thesis the focus is on carrier-LO-phonon collisions providing an efﬁcient mech-anism to populate the QD states. The main difﬁculty in combining the quantum kinetics for carrier scattering and the luminescence dynamics lies in the different timescales on which the underlying processes take place. Carrier scattering processes typically occur on a ps timescale, whereas recombination processes are in the order of 1 ns. Hence, some

approximation for the carrier-scattering processes in the luminescence model is affordable and we might employ the relaxation time approximation

d
dtf_{α}

coll =−f_{α}−F_{α}

τ_{α} . (6.25)

Close to the quasi-equilibrium/steady-state population F_{α}, the Markov approximation is
valid. In a ﬁrst step, we extract the relaxation timesτ_{α}from a quantum-kinetic calculation
for an initially empty QD-WL system where carriers are excited optically into the WL.
Us-ing these relaxation times, in a second step Christopher Gies performed the calculation of
the time-resolved PL signal from the SLE including correlations as outlined above.
Specif-ically, we considered an unstructured sample where stimulated emission is absent. The
corresponding results are shown in Fig. 6.4, including a comparison with experiments
per-formed by Gareth Beirne in the group of Prof. Peter Michler at the University of Stuttgart.

(a) experiment (b) theory

**Fig. 6.4: Time-dependent PL signal of a single InP/InGa**_{0.51}P_{0.49} semiconductor QD
ob-tained from experiment and theory [173].

The experimental results for the s-, p- and d-shell emission lines of a single InP QD at 4 K are presented in Fig. 6.4a. In general, all of the transients show a fast rising time and a non-exponential decay. Furthermore an increasingly delayed PL intensity maximum with increasing power density and a larger width of this maximum for the s-shell than for higher shells is observed. The behavior of the PL maximum originates from the ﬁlling of lower-lying levels from occupied higher levels. Due to successive relaxation, the d-shell reaches its PL maximum earlier than the s-shell. Even for late times the s-shell population is still feeded by higher shells, resulting in the broader PL maximum.

For the microscopic analysis we restrict ourselves to a InP/InGaP QD system with two conﬁned shells, s- and p-shell, for electrons and holes. The level spacing is chosen in such

a way that for low-density excitation conditions a phonon bottleneck for the scattering to the lowest conﬁned electron state is predicted by perturbation theory. It turns out that the results from the microscopic analysis, depend only weakly on the exact values used for the level spacing. In the example shown in Fig. 6.4b, we chose a level spacing of 34.4 meV for electrons and 9.6 meV for holes, whereas the LO-phonon energy is 46 meV. Other material parameters are summarized in Tab. B.1.

In a ﬁrst step we consider the optical excitation in the WL and neglect carrier
recombi-nation. From the quantum kinetic calculation (cf. Chap. 5.2.2 for InGaAs QDs) we ﬁnd
efﬁcient carrier relaxation for the present low-temperature conditions (10 K). The
evolu-tion towards a steady-state populaevolu-tion can be approximately described by a relaxaevolu-tion time
ofτ_{e}=3.5 ps for electrons andτ_{h}=1.5 ps for holes. These relaxation times are effective
val-ues, considering all of the possible inward and outward scattering processes. Note, that
for elevated excitation densities also carrier-carrier interaction contributes to fast
scatter-ing processes, while at low carrier densities the effects due to carrier-phonon interaction
discussed above are expected to dominate.

The luminescence dynamics calculated according to the theory outlined above are shown in Fig. 6.4b. To mimic the ﬁnite temporal resolution of the experimental setup of about 35 ps, we convoluted the results with a corresponding Gaussian-shaped apparatus function.

First, due to fast carrier relaxation, a rapid rise of the PL intensity is observed. From our quantum kinetic calculation we ﬁnd practically the same relaxation time for the s- and the p-shell. Therefore, similar rise times are expected in the PL signal, which is also observed in the experiment. The initial decay of the PL signal from the p-shell is faster, because, in addition to recombination, carrier relaxation to the s-shell further reduces the p-shell population. At later times when the QD is populated, the PL intensity decays as spontaneous recombination processes reduce the population. The decay of the PL signal reveals a non-exponential signature. This is due to the fact that in semiconductor QDs electrons and holes are not fully correlated, in contrast to atomic systems where an electron in the excited state implies that there is a hole in the lower state.

The non-exponential decay can be understood analytically. Neglecting Coulomb
correla-tions and adiabatically solving Eq. 6.24, we ﬁnd from Eq. 6.22 that for example the loss of
conduction-band carriers due to spontaneous recombination is given by _{dt}^{d}f_{α}^{c} =−^{f}^{α}^{c}^{(1−f}_{τ}_{α} ^{α}^{v}^{)}.
Hence, as long as the valence-band population is not ﬁxed, for example by background
doping, a non-exponential behavior is observed due to the fact that the temporal evolution
of conduction-band and valence-band states might be different.

In recent years an increasing interest in nitride-based semiconductor nanostructures evolved.

For practical applications they have several advantages in comparison to GaAs materials or II-VI compounds. As can be inferred from Fig. 7.1, this material system allows for light sources with emission frequencies ranging from amber to the UV. A famous exam-ple is the ﬁrst blue GaN-based laser diode demonstrated by Nakamura [174]. Nowadays, blue and green nitride LEDs are widely used in full-color LED displays and trafﬁc lights.

Nitride laser diodes emitting at 405 nm are for example implemented in the upcoming Blu-ray players. More applications and a detailed introduction into nitride semiconductors are presented in Refs. [175–178].

**Fig. 7.1: Bandgap vs. lattice constant. Picture taken from Ref. [179] (Reprinted with**
permission, Copyright 2003, American Institute of Physics).

Nitrides are a challenging material system, in the experiment as well as for the theoretical description. Their compounds crystallize either in a meta-stable zincblende phase [180]

or in the stable wurtzite structure, depending on growth conditions and the substrate. For optoelectronic devices usually the wurtzite structure is used and therefore we restrict the following discussion to this phase. The crystal growth is accompanied by various types of defects, dislocations, and segregation [175, 176], which complicate the fabrication of

nanostructures like quantum dots or Bragg-reﬂectors in good crystalline quality. For the theoretical description most challenges arise from the wurtzite crystal structure. The crys-tal structure is of central importance for the understanding of the electronic and optical properties as it implies the symmetry properties of the wave-functions. Additionally, one has to account for example for a non-parabolic dispersion, a pronounced mass anisotropy, and built-in electrostatic ﬁelds [179, 181]. As a consequence, many of the approximations working well for zincblende GaAs materials are not applicable to the nitride system.

(a) wurtzite (b) zincblende

**Fig. 7.2: Conventional unit cell of GaN in zincblende and wurtzite phase (picture courtesy**
of N. Baer [140]).

One important consequence of the crystal symmetry are intrinsic electrostatic ﬁelds due to
spontaneous and strain-induced polarization. The unstrained zincblende structure shown
in Fig. 7.2b is non-polar. Its inversion symmetry ensures that polarizations due to different
bond lengths are compensated, see for example Ref. [178]. In contrast, even the unstrained
wurtzite lattice shown in Fig. B.1a exhibits a polar axis inc-direction. The geometry of the
conventional unit cell usually deviates from the ideal ratio of _{a}^{c} =2

8/_{3}[182], resulting in
a so-called spontaneous polarization inc-direction. Beside the spontaneous polarization,
large strain-induced piezoelectric ﬁelds (1-10 MV/cm) are observed [179, 183, 184],
es-pecially in heterostructures like QDs and QWs. In a QW, the resulting electrostatic ﬁelds
give rise to a separation of electron and hole wavefunction, also known as the
quantum-conﬁned Stark effect (QCSE) [185]. As the charge separation implies a reduction of dipole
transitions, many investigations for QWs [48, 186] and QDs [47, 49] were devoted to this
effect. For device application, several approaches have been developed to circumvent these
internal ﬁelds. Among them are for example the growth on the non-polara- andm-planes
[187, 188] or strain-engineering by using lattice-matched quaternary alloys [189].

Much work has been devoted to study the electronic properties of group-III nitrides [179].

Basically three approaches are available: continuum**k**·**p**models, atomistic tight-binding

(TB) models, and density-functional theory (DFT) calculations. Even on nowadays
super-computers DFT calculations are restricted to a few hundred atoms, and hence this method
is not appropriate to study QDs. In the following, basically TB calculations are used. A
comparison of the TB approach with a**k**·**p**model is subject of current research [190].

In previous chapters of this thesis weak polar coupling InGaAs QDs have been investi-gated. Polaron renormalizations and their inﬂuence on carrier scattering and optical ab-sorption spectra were studied. For this discussion, the nitride material system provides new interesting aspects. Stronger polaron effects are expected due to the intermediate po-lar coupling. Furthermore, the inﬂuence of material properties like piezo-ﬁelds and strong band-mixing effects on polaron renormalizations, carrier scattering, and optical properties is of particular interest.

To study the inﬂuence of a stronger polar coupling and speciﬁc material properties, two ap-proaches are followed in this chapter. In a ﬁrst step the inﬂuence of the built-in electrostatic ﬁelds and the intermediate polar coupling is estimated within an effective-mass model. In a second step a much more detailed study is presented. We start from an atomistic empiri-cal TB approach for the single-particle states. This is combined with the GF theory for the carrier kinetics and the inﬂuence of polaron renormalizations on optical spectra is studied as a ﬁrst application of this method.

**7.1 Envelope wave function model**

The most striking differences between GaN and GaAs QDs are a larger polar coupling and the presence of intrinsic electrostatic ﬁelds. In the following chapter, their inﬂuence on the polaron renormalizations and the carrier scattering is investigated. In a ﬁrst approach we restrict the analysis to an effective mass approximation and use the envelope wave-function model discussed in Chap. A.1. The calculation of the energy dispersion for the WL states is more involved. Especially for holes, a strong band-mixing of the heavy-hole and the light-hole band occurs, resulting in non-parabolic bands and a strong mass anisotropy [179, 181].

However, the inclusion of such effects is the subject of Chap. 7.2–7.4. Here, they are not considered.

Very controversial values have been reported for the spontaneous polarization as well as for
the elastic constants that determine the strain-induced contribution. For InGaN
nanostruc-tures that are embedded compressively strained in GaN, the resulting intrinsic electrostatic
ﬁelds amount to a few MV/cm [179, 183, 184]. Therefore, we consider typical values
of +2.0 MV/cm inside the QD-WL region and -0.5 MV/cm in the surrounding GaN. A
detailed summary of the material parameters for the In_{0.2}Ga_{0.8}N alloy we consider is
pre-sented in Tab. B.2.

**Quantum-conﬁned Stark effect**

The carrier conﬁnement together with the built-in electrostatic ﬁelds gives rise to the so-called quantum-conﬁned Stark effect (QCSE). Using the separation of the envelope wave function (A.1), the electrostatic ﬁelds only inﬂuence the component in growth direction.

The corresponding one-dimensional Schrödinger equation is given by

− ^{2}
2m

∂^{2}

∂z^{2} +U(z)

ξ(z) =E(z)ξ(z), (7.1) where the potential

U(z) =U_{0}(z) +U_{p}(z) +U_{scr} (7.2)
contains the conﬁnement potentialU_{0}(z), the potential due to the electric ﬁeldU_{p}, and the
potential of the screening ﬁeldU_{scr}due to the spatial separation of electrons and holes. The
screening potential

U_{scr}(z) = e^{2}N
2ε_{0}ε_{b}

dz^{} |ξ^{e}(z^{})|^{2}− |ξ^{h}(z^{})|^{2}

|z−z^{}| (7.3)

is calculated by solving Poisson’s equation for a set of uniformly charged sheets.

-0.5 0 0.5 1

0 0.2 0.4 0.6 0.8 1

-12 -8 -4 0 4 8 12

z in nm

-1 -0.5 0

confinement potential in eV

0 0.2 0.4 0.6 0.8 1

wavefunction |ξ(*z*)|2

b) a)

**Fig. 7.3: Quantum conﬁned stark effect due to intrinsic electrostatic ﬁelds in growth **
direc-tion for electrons (a) and holes (b).

The spontaneous polarization of the GaN matrix and of the strain-induced polarization of InGaN QD have different magnitude and opposite sign. This gives rise to a consequence, a sawtooth proﬁle of the band structure in z-direction, similar to a set of capacitors with non-equal surface charges [183, 191]. Corresponding results from a self-consistent solu-tion of the Schrödinger-Poisson equasolu-tion (7.1)–(7.3) are shown in Fig. 7.3. Due to the tilted conﬁnement potential a spatial separation of charges is observed. This has several

consequences. Less effective interband processes are expected due to the reduced overlap of electron and hole wave functions in the corresponding matrix elements. On the other hand, intra-band interaction matrix elements remain almost unchanged.

**Nitride polaron**

In comparison to InGaAs QDs, stronger polaron effects are expected in GaN QDs due to the lager polar coupling. The polaron renormalizations for nitride QDs are calculated similar to the InGaAs material. As discussed in detail in Chap. 5.1, the corresponding Dyson equation for the retarded GF is solved in the time domain and the spectral function is obtained by Fourier transformation.

10^{-6}
10^{-4}
10^{-2}

10^{0} (a) WL (k=0)

10^{-6}
10^{-4}
10^{-2}
10^{0}

-2 Im *G*R (ω)

(b) QD p-shell

-4 -2 0 2

Energy (h* ^{_}*ω

*- E*

_{G}) / h

*ωLO*

^{_}10^{-6}
10^{-4}
10^{-2}

10^{0} (c) QD s-shell

**Fig. 7.4: Polaron spectral function for InGaN QDs at 300K.**

For the discrete QD states, the spectral function in Fig. 7.4 shows that the free-particle picture is strongly modiﬁed. On this level, a direct comparison between the the weak-polar coupling material system InGaAs (Fig. 5.2) and the InGaN system with intermediate polar coupling is possible. In the ﬁrst case, one can clearly distinguish between phonon

replicas of the QD states which are spaced by the LO-phonon energy ω_{LO} around the
central peak, and the hybridization effect which leads to a splitting of these peaks that is
smaller than the LO-phonon energy (when the detuning between the QD level spacing and
the LO-phonon energy is small). In the InGaN material system, the hybridization is much
stronger and one can no longer distinguish between phonon replicas and their splitting.

Moreover, the obtained rich multi-peak structure provides a stronger overlap between the spectral functions which increases the scattering efﬁciency discussed below. Broadening of the resonances is provided by the coupling to the WL states and the ﬁnite LO-phonon lifetime (assumed to be 5 ps).

**Consequences for carrier-LO-phonon scattering**

The scattering mechanism including polarons is discussed extensively in Chap. 5.2.2 for
the weak polar coupling InGaAs material. In QD systems, the spectral functions are of
central importance, since their overlap basically determines the scattering efﬁciency
be-tween two particular states. As shown above, large polaron renormalizations are found in
the intermediate polar coupling regime. Their inﬂuence on the carrier scattering in nitride
QDs, together with the intrinsic electrostatic ﬁelds, is subject of the following discussion
In a ﬁrst example, we study the capture of WL carriers into QD states and the relaxation
of QD carriers for a given WL population. The time evolution of the occupation function
for s- and p-shell is shown in Fig. 7.5a. As initial condition we use empty QD states
and a thermal population of the WL states that corresponds to a carrier density10^{10}cm^{−2}.
For a situation where for electrons the level-spacing is1.2ω_{LO}, fast scattering processes
are observed which lead to capture times of 1.07 ps and 1.02 ps for s- and p-shell,
re-spectively. As discussed in Chap. 5.2.1 for the InGaAs material, the fast carrier scattering
is due to quasi-particle renormalizations which strongly modify the picture of scattering
between free-carrier states as well as due to memory effects. Our ﬁnding of a weak
de-pendence of the ultrafast redistribution of carriers on the detuning between level spacing
and LO-phonon energy in weak polar coupling materials (cf. Chap. 5.2.1) remains true
for intermediate polar coupling nitride materials. The inﬂuence of the built-in electrostatic
ﬁeld on the carrier dynamics turns out to be weak, since the charge separation only weakly
modiﬁes the matrix elements for intra-band scattering processes.

Another example is the carrier scattering after optical excitation in the p-shell. In Fig. 7.5b
corresponding results are presented for a QD with a level-spacing of 1.2ω_{LO}for electrons
and 0.4ω_{LO} for holes. Due to pulse excitation, ﬁrst the p-shell is populated. The carrier
relaxation is so fast that already during the optical pulse a strong redistribution from the
p-shell to the s-shell takes place. As the ultrafast scattering processes are connected with
strong dephasing of the coherent interband polarization, which is included on the same
quantum-kinetic level as the carrier scattering, the time evolution of the interband
polar-ization practically follows the optical pulse (not shown). Correspondingly, the coherent

0 0.2 0.4 0.6 0.8 1 1.2

Time in ps

0 0.002 0.004 0.006 0.008 0.01

Population

0 MV/cm 2 MV/cm

p-shell s-shell

(a) capture from WL and relaxation

0 0.5 1 1.5 2

Time in ps 0

0.0005 0.001 0.0015

0.002

Population

p-shell s-shell

(b) relaxation after optical excitation of the p-shell

**Fig. 7.5: Inﬂuence of the QCSE on the temporal evolution of the QD population which is**
initially empty due to (a) capture and relaxation of WL carriers and (b) optical excitation
of carriers in the p-shell.

regime is limited to the duration of the 100 fs pump pulse. During the coherent regime a transient strong increase of the total carrier density is obtained. While relaxation, the time-domain oscillations in Fig. 7.5b indicate the strong coupling between carriers and phonons and the oscillation frequency is connected to the hybridization in the DOS as discussed in Chap. 5.2.1. Note that the oscillations appear after the optical pump pulse in the incoherent regime and hence they are not connected to optical coherence. At larger times, the possi-bility of carrier transitions between QD and WL states leads to a redistribution of carriers from the QD states into the WL. Of course, the total carrier density remains constant after the pulse.

The ultrafast scattering and dephasing processes are the direct result of the polaronic renor-malizations. Only within a non-Markovian calculation the above mentioned oscillations in connection with the strong-coupling regime for the carrier-phonon interaction can be obtained. In this respect, there is no qualitative difference between the InGaAs and InGaN material systems. But in the latter case, the larger polar coupling increases the scatter-ing efﬁciency, while the electron and hole charge separation induced by the built-in ﬁelds reduces only inter-band but not intra-band processes. We restricted the analysis to low carrier densities and the interaction with LO phonons. At elevated excitation densities, carrier-carrier scattering additionally contributes. A detailed discussion of this topic is be-yond the scope of this thesis. Nevertheless, corresponding studies are presented by Nielsen et al. [91, 92, 192].